HAL Id: hal-01876621
Submitted on 18 Dec 2019
HAL is a multi-disciplinary open access
archive for the deposit and dissemination of
sci-entific research documents, whether they are
pub-lished or not. The documents may come from
teaching and research institutions in France or
abroad, or from public or private research centers.
L’archive ouverte pluridisciplinaire HAL, est
destinée au dépôt et à la diffusion de documents
scientifiques de niveau recherche, publiés ou non,
émanant des établissements d’enseignement et de
recherche français ou étrangers, des laboratoires
publics ou privés.
Effect of chemical and thermal activation on the
microstructural and mechanical properties of more
Omar Abdulkareem, Amor Ben Fraj, Marwen Bouasker, Abdelhafid Khelidj
To cite this version:
Omar Abdulkareem, Amor Ben Fraj, Marwen Bouasker, Abdelhafid Khelidj.
chemical and thermal activation on the microstructural and mechanical properties of more
sustainable UHPC. Construction and Building Materials, Elsevier, 2018, 169, pp.567-577.
Effect of chemical and thermal activation on the microstructural and
mechanical properties of more sustainable UHPC
Omar M. Abdulkareema,b,c
, Amor Ben Fraja,⇑
, Marwen Bouaskerd
, Abdelhafid Khelidjb
Cerema, Project-team DIMA, 120 rue de Paris, 77171 Sourdun, France
Lunam University, University of Nantes, IUT Saint-Nazaire, GeM, UMR CNRS 6183, 58 rue Michel Ange, BP 420-44600, Saint-Nazaire, France
University of Mosul, College of Engineering, Department of Environmental Engineering, 41002 Mosul, Iraq
University of Orléans, University of Tours, INSA Centre Val de Loire, LaMé, 8 rue Léonard de Vinci, 45072 Orléans, France
This paper investigates the influence of the content of blast furnace slag (BFS) on the microstructural and mechanical properties of non-activated and activated ultra-high performance concrete (UHPC). Three volume-substitution rates of cement with BFS were explored (30% for UHPC2, 50% for UHPC3and 80%
for UHPC4) and two activation methods, chemical and thermal, were tested. Results show that with
30% of BFS, heterogeneous nucleation prevailed over dilution, accelerating the hydration reaction of cement and increasing the amount of C-S-H formed. C-S-H decreased the porosity of UHPC2by 18%
and 20% respectively at 3 and 90 days. The compressive strengths of UHPC1(without BFS) and UHPC2
were very similar. For high BFS contents, the dilution effect prevailed and there was less portlandite, which decreased the amount of hydrated products, particularly at early age. As a result, the porosity of UHPC3and UHPC4was more than twofold higher than that of UHPC1.
To boost the hydration reaction of blended UHPC with a high BFS content, KOH was added. The use of [KOH]3significantly increased the amount of hydrated products, reducing the porosity of UHPC41.6-fold
at 3 days and increasing its compressive strength by 42% at the same age. However, this activation mode was not enough to ensure the required compressive strength of UHPC1. Thermal activation at 90°C for 2
days was therefore tested. Results showed the acceleration of the reaction of solid components, which increased the consumption of portlandite and hence the development of hydrated products. This resulted in improving the packing density of blended UHPC, decreasing its porosity and enhancing its compressive strength. In comparison with reference concrete at 90 days, the compressive strength of UHPC3-T
increased by 7% and that of UHPC4was 12.5% lower.
Since the 1980s, specialized applications that demand greater strength and corrosion resistance triggered research to develop a concrete with an extremely high strength and dense
microstruc-ture , that subsequently led to the development of ultra-high performance concrete (UHPC). Ultra-high performance concrete is a distinctive cement-based substance that behaves like a minimal-porosity ceramic material with enhanced mechanical properties . This concrete is distinguished by a grain size of the ingredients (cement, silica fume, crushed quartz, quartz sand) that does not exceed 600mm, a low water-to-binder ratio (w/b) and a high content of water reducer (superplasticizer). By virtue
⇑ Corresponding author.
of both the highly dense (specific gravity ranges over 2500–3000 kg/m3) and homogenous microstructure of UHPC, its typical
strength can reach 150–200 MPa in compression, 7–15 MPa in uni-axial tension, and 25–40 MPa in bending[4,5]. This exceptional performance is due to its higher cement content, lower w/b, inte-gration of silica fume and low CaO/SiO2 ratio. On account of
its extraordinary compressive strength, UHPC exhibits great sensi-tivity to certain parameters such as the quality of cementitious composites, quality of curing (standard or heat treatment), particle size of aggregate and the applied production techniques, etc. Richard and Cheyrezyreported that if soft cast and cured at ambient conditions, its compressive strength (CS) can reach 200 MPa, and that CS values exceeding 800 MPa can be attained when pressure molding is adopted. Hence, the weight of a structure built solely with UHPC can be reduced by one-third to one-half in com-parison to that with a traditional reinforced concrete structure under the same load [2,8]. Mounanga et al.  ascribed this improvement in mechanical behavior to a better cement hydration and a close granular packing of the UHPC with the addition of crushed quartz. Crushed quartz particles have a high specific area, which improves the homogeneity and the packing density of con-crete. From the porosity standpoint the collateral effect of hydra-tion on porosity is as follows: due to the low w/c, the capillary porosity decreases and the Interface Transition Zone (ITZ) is filled up with C–S–H hydrates generated by the pozzolanic reaction of silica fume. The pore size of UHPC essentially ranges between 2 and 3 nm, the most frequent pore size being 2.0 nm, and its total porosity is 2.23%.
Despite the high mechanical performance of UHPC, its manufac-ture involves a high energy consumption. The energy required for cement production is around 1700–1800 MJ t clinker, which is the third largest consumed energy, after that of the aluminum and steel manufacturing industries. The high quantity of cement in UHPC (over 800–1000 kg/m3) has a detrimental impact on the
hydration heat and may create shrinkage deformations, which decrease the hardened performance by microcracking. Besides, it displays downsides from the economic and sustainability stand-points.
Portland cement is responsible for 74–81% of global CO2release
as each 1 kg of cement produced generates around of 0.9 kg of CO2.
This equates to about 3.24 billion tons of CO2yearly. Taking
into consideration both the boosted mechanical properties of UHPC and its high environmental influence, it appears worthwhile explor-ing a path to produce UHPC with a low environmental footprint.
Blast furnace slag (BFS) is one of the industrial co-products that can substitute for Portland cement to a certain extent. The use of this alternative material depends mainly on the availability and the domain of application. The major components of BFS are CaO, SiO2, Al2O3and MgO. It is categorized as a potential hydraulic
mate-rial (reaction with water) rather than a pozzolanic one (reaction with lime), despite its slow reaction with water[15,16]. This latent hydration reaction restricts the strength development of concrete at early age. However, at later age, the microstructure is more refined, porosity is lower and consequently the mechanical perfor-mance of blended concrete is enhanced, in comparison with that of Portland cement. Thanks to its high specific area and its chemical composition, BFS has a double effect on the behavior of UHPC, both physical and chemical. The physical effect consists in (i) the dilution induced by the substitution of cement with BFS, which increases the water-to-cement ratio; (ii) the filler impact due to the fineness of BFS particles, improving the packing density of the mixture; (iii) the stimulation effect, as the BFS particles act as nucleation sites, accelerating the cement hydration reaction. This results in the production of portlandite, which reacts with BFS to form hydrates.
Yu et al.revealed that in presence of slag, the portlandite content of UHPC decreased, denoting its consumption by BFS to
form dense C-S-H. The latter fills the pore structure, which results in a compressive strength enhancement of blended UHPC. Other studies have found that increasing the BFS content (70%) increases the portlandite consumptionwithout improving the concrete performance. Zhou et al.observed that the higher the quantity of slag, the higher the total porosity. This can be explained by the very low cement content, which restricts the formation of port-landite. The latter is responsible for promoting the hydration reac-tion of BFS.
The decrease in mechanical performance of slag-blended UHPC particularly concerns the early age, as the strength development is decelerated by the latent reaction of BFS. Yazici et al. mea-sured a higher drop of compressive strength at 2 days when the slag replacement rate reached 40%, while at 28 days the compres-sive strength was close to that of reference UHPC. Gupta 
reported a decrease in early compressive and flexural strengths with 40 and 60% of slag, whereas a growth in later strength was measured even with 80% of slag content. Shi et al.also found that at 3 days, the compressive strength of UHPC decreased from 84 MPa to 78 MPa when 25% of cement was substituted with slag. At 56 days, the compressive strength reached 125 MPa.
Accordingly, since slag itself is nothing more than a latent hydraulic binder with lower early strength and longer setting time, its hydration reaction needs to be boosted. This can be achieved by chemical or thermal activation. Among chemically activated binder systems, alkali activated slag (AAS) is one of the most widespread substances thanks to its lesser environmental effect, quick setting, and swift early strength gain. In presence of an alkali activator (such as sodium or potassium hydroxide), the hydroxyl ions (OH) -accelerate the hydration reaction by enhancing dissolution of the aluminate and silicate network in the slag to form calcium silicate hydrates with a high amount of Al2O3(C-A-S-H). This increases the
early compressive strength[24–26], depending on different factors such as the activator dosage and the interactions between con-stituents[25,27–29].
As already mentioned, chemical activation is used with ordinary cementitious materials and there has been no research into its effect on UHPC properties. Some research has been carried out, however, on thermally-activated UHPC, mainly in presence of min-eral admixtures. Slag, thanks to its higher activation energy, is par-ticularly sensitive to thermal activation[30–32]which accelerates the pozzolanic reaction, increasing the amount of hydrated prod-ucts and densifying the microstructure even further. As a result, the compressive and flexure tensile strengths will be higher
[1,33]. Bougara et al.measured an increase in compressive strength at early age for mixtures with 30% and 50% of slag when the temperature rose from 20°C to 40 °C and 60 °C, whereas the strength at later age decreased. The same trend was observed by Castellano et al., who measured a great increase in early com-pressive strength when the temperature was raised from 20°C to 40 and then to 60°C. After 7 days the trend was reversed. On the contrary, Sajedi et al. showed that the 90-day compressive strength of mortar with 50% of slag, treated at 60°C for 20 h, exceeded that of reference mortar by circa 12%.
In conclusion, despite the various studies carried out on UHPC, none have dealt with chemical activation and its effect on UHPC properties, and few of them correlate the thermal activation with the microstructural change, in order to explain the mechanical behavior of UHPC, particularly in presence of slag.
2. Research objective
This paper deals with the effect of BFS content on the microstructural and mechanical properties of non-activated and activated UHPC. The research was carried out at two scales: the
micro-scale, by (i) assessing the different phases resulting from the hydration reaction, and (ii) assessing the porosity, and the macro-scale, by studying the mechanical properties of manufactured UHPC. To highlight the latent reaction of BFS and the interest of chemical and thermal activation in improving blended-UHPC prop-erties, the mechanical properties were measured at 3 and 90 days, and the results were correlated with the state of the microstruc-ture at the same ages.
3. Experimental program 3.1. Materials and mixtures
The materials used to manufacture the concrete were of local origin (France): the cement CEM I 52.5 PM ES comes from Le Teil plant, the grey Silica Fume (SF) is marketed by Condensil as S95 B DM, the Blast Furnace Slag (BFS) comes from Ecocem, the Crushed Quartz (CQ) and Quartz Sand (QS) are marketed by Sibelco as C500 and CV32, respectively. The chemical properties of these components are detailed in. Their physical properties are pre-sented inTable 1.
To ensure the high workability of manufactured UHPC, a Sika Viscocrete Krono HE 20 superplasticizer (SP) was added. It is a high-range water reducer with a density and solid content of 1.085 and 41%, respectively. The content of this acrylic copolymer was adjusted to ensure the same slump flow for all UHPC regard-less of their BFS content. All formulations had the same water con-tent (considering the water brought by the superplasticizer) and only BFS and SP contents were varied (Table 2). The optimization of these concrete mixtures is detailed in.
Solid components were incorporated in an intensive 15 L Eirich mixer and mixed for 30 s. Then dissolved superplasticizer and water were added and mixed with the other materials for 3 min to ensure a homogeneous mixture, except for UHPC with KOH. For the latter, the mixing time was extended by 30 s to ensure the required slump flow. After mixing, the concrete was poured into steel molds, stored for 24 h before demolding, and plastic-wrapped, to avoid any drying. Subsequently, the specimens were stored in a fog room at 20°C for 3, 7, 28, and 90 days.
3.2.1. Chemical activation
The use of mineral additions, in particular BFS, decelerates the hydration kinetic of concrete and induces a decrease in its early age properties, as the substitution of cement decreases the alkali content of concrete. Alkalis promote the reaction of BFS by destroy-ing its chemical bonds and acceleratdestroy-ing its reaction with water, thereby increasing its strength. To compensate for this lack of alka-lis, KOH can be added, but its addition may have a negative effect on the environment and should be strictly controlled.
Considering the quantity of alkalis in cement (0.24%), we calcu-lated the quantity of alkalis lost when cement is substituted with BFS and then the quantity of KOH required to compensate for these lost alkalis. This first concentration is called [KOH]1 and equals
3.39 kg/m3 (3.39 g/l of concrete). This concentration was then
increased two ([KOH]2) and three ([KOH]3) times to improve the
early age compressive strength of UHPC, without affecting its workability, by maintaining a slump flow of 300 mm. The opti-mization of this concentration is detailed in.
3.2.2. Thermal activation
Thermal activation is employed to accelerate the maturing of concrete, for an equivalent age. The latter corresponds to tT= tx
t0,where t0and txare respectively the time of water/binder contact
and the theoretical time to obtain the same level of concrete matu-rity in the case of conservation at 20°C.
Generally, the level of maturity depends on hydration reactions and their rate of progress (n). The evolution of n versus tempera-ture was approximated with Arrhenius’ law, applied on all the hydration reactions of cement:
n ¼dn dt¼ ~AðnÞ exp Ea RT ð1Þ where ~A is the chemical affinity,n the rate of progress of hydration reactions, Eathe activation energy (J mol1), R the perfect gas
con-stant (8.314 J mol1K1) and T the temperature of the concrete throughout the test.
To estimate the equivalent age tTfor moderate thermal
treat-ments, equation 1 was integrated between initial (tinitial) and final
(tfinal) times, as:
tT¼ Z tfinal tinitial exp Ea R 1 293 1 TðtÞ dt ð2Þ
tTwas approximated as:
tT¼ Xn i¼1
Dti exp Ea R 1 293 1 TðtÞ ð3Þ where tTis the equivalent age for the chosen temperature;Dti, the
duration of concrete exposure to Ti; Ti, the temperature of concrete
duringDti, in Kelvin; Ea, the activation energy and R, the perfect gas
For simplification, Eais considered as constant and resulting
from all the hydration reactions of the binder; Ea/R is 4000 K and
6000 K for CEM I and CEM III, respectively[38,39]. For this study, a high BFS content was explored (up to 62% of whole binder). Thus, the binder was assimilated to composed cement, CEM III. Thermal activation was applied particularly to concretes with a high BFS content (UHPC3and UHPC4) in order to ensure the same long term
properties as UHPC1. Therefore, the equivalent age should be more
than 90 days. As shown in Fig. 1, a temperature of 90°C was applied, 24 h after mixing, for 2 days, before testing UHPC. This results in activated UHPC, with an equivalent age of 103 days. 3.2.3. Thermogravimetric analysis
This test used a thermal analyzer instrument NETZSCH STA 449 F3under dynamic nitrogen atmosphere and carried out on 250 mg
powdered samples heated from 30°C to 1250 °C at a rate of 10 °C/ min. At a testing age of 3 and 90 days, the specimens were crushed (<315mm) and hydration was stopped by immersion in methanol. The outputs of the test are the loss in mass per degree Celsius and
Fineness and density of solid components.
CEM I 52.5 SF QQ BFS QS Specific area (cm2 /g) 3555* 250,000** 10,435* 4450* 124* Density (–) 3.17 2.24 2.65 2.90 2.65 * Blaine. ** BET.
the differential thermogravimetric (DTG) curves. The mass loss due to the liberation of bound water (H), decomposition of portlandite (CH), and liberation of CO2was measured at the respective
temper-ature intervals and the accurate limits for the tempertemper-ature inter-vals were specified considering the derivative thermogravimetric curves (DTG). The mass loss of bound water through dehydration of some hydrates (C-S-H, ettringite, etc.) occurred between 180 and 300°C, while that corresponding to the dehydration of port-landite occurred between 450 and 530°C. The decarbonation of calcium carbonate took place between 700 and 900°C.
3.2.4. Total porosity
The Mercury Intrusion Porosimetry (MIP) test was carried out on 1 cm3 samples at 3 and 90 days. At 3 days, samples were
immersed in methanol to stop the hydration reaction, before dry-ing at 105°C and testing.
3.2.5. Mechanical properties
Flexural and compressive strength tests were carried out on 40 40 160 mm prism specimens at 3, 7, 28 and 90 days, according to NF EN 196–1. A press machine of 300 kN was used, with loading speeds of 0.05 kN/s and 2.5 kN/s respectively for flexural and com-pressive tests. Each strength is the average of three samples’ strength. The splitting tensile strength was measured on cylindri-cal specimens 110 mm in diameter by 220 mm in height at 3 and 28 days. The specimens were tested using a 2000 kN-press machine. For each mixture, two cylinders were tested and the mean value is reported.
4. Results and discussion 4.1. Thermogravimetric analysis
The TGA and DTG curves of whole UHPC mixtures after hydrat-ing for 3 and 90 days are presented in Figs. 2–5, respectively.
Table 3 shows the variation in content with hydration times of portlandite and calcite beside the amounts of chemically bound water for whole UHPC mixtures.
4.1.1. Effect of BFS content
The TGA curves ofFig. 2exhibit the mass loss for the hydrated UHPCs at 3 days, in the following sequential order: dehydration, dehydroxylation or calcination of remaining ettringite, portlandite
Composition of studied UHPC mixtures.
) UHPC1 UHPC2 UHPC3 UHPC4 UHPC4-[KOH]3
CEM I 977.00 683.90 488.50 195.40 195.40 SF 183.00 183.00 183.00 183.00 183.00 QQ 61.00 61.00 61.00 61.00 61.00 BFS – 268.10 446.90 715.00 715.00 QS 1075.00 1075.00 1075.00 1075.00 1075.00 SP 25.31 10.54 22.49 25.31 25.31 W 145.63 160.39 148.44 145.63 140.65 KOH – – – – 10.17 Slump Flow (mm) 300
Fig. 1. Thermal activation mechanism.
-7 -6 -5 -4 -3 -2 -1 0 0 300 600 900 1200 UHPC1 UHPC2 UHPC3 UHPC4 Temperature (°C) Mass loss %)
Fig. 2. TGA for UHPC mixtures at 3 days.
-0.3 -0.2 -0.1 0 0.1 0 300 600 900 1200 UHPC1 UHPC2 UHPC3 UHPC4 DTG (%/mi n) Temperature (°C)
Fig. 3. DTG for UHPC mixtures at 3 days.
-10 -8 -6 -4 -2 0 0 300 600 900 1200 UHPC1 UHPC2 UHPC3 UHPC4 Temperature (°C) Mass Loss (%)
decomposition and calcite decarbonation. It can be noted that all the tested specimens demonstrate a comparable trend of mass loss. Nonetheless, the rates of their mass loss in each temperature range are dissimilar, indicating that the quantity of material react-ing at each treatment stage differs and depends on the percentage of slag used to substitute for cement, in particular when this reached 80% in UHPC4. The results show that the higher the slag
content, the lower the measured mass loss. This can be clearly seen inTable 3through the difference in mass loss percentages between UHPC1 and UHPC4 at 3 days: the chemically bound water
decreased from 3.3 % to 2.1%, portlandite from 1.42% to 0.35%, and calcite from 3.9% to 2.8%, respectively. Generally, the incorpo-ration of slag in cement generates a lower quantity of portlandite in the hydration product due to the impact of dilution in addition to the consumption of portlandite through the pozzolanic reaction
. When portlandite forms during cement hydration, some of this compound is consumed by the pozzolanic reaction of silica fume and slag reaction and this consumption is increased when the amount of slag is increased, inducing a delay in concrete hydra-tion and forming supplemental C-S-H. Thus, the mass loss of portlandite in the blended mixtures of UHPC is the least at early ages when compared to UHPC1. Likewise, the results show that
the substitution of Portland cement with slag diminishes the quan-tity of C-S-H and C-A-H formed at 3 days in comparison with UHPC1. The quantification of phases related to mass change for
the UHPC mixtures was accompanied by the occurrence of major peaks in the DTG curves, as shown inFig. 3. The prominence of these peaks can be attributed to the evaporation of free water, portlandite and calcite decompositions, sequentially. The endothermic peak of both C-S-H and ettringite decreases with increasing slag content. The decrease of the portlandite content in the UHPCs containing slag restricts the promotion of the slag pozzolanic reaction, and the already-produced pore structure in these blended mixtures cannot be filled by the recently produced C-S-H.
As expected, the content of chemically bound water in the UHPC mixtures increases remarkably at 90 days, as shown in
Table 3. The measured mass loss of the UHPC mixtures also
increases with increasing age up to 90 days, indicating a continu-ing hydration with time as demonstrated inFig. 4. The mass loss of portlandite remains lower in the UHPC mixtures containing slag compared to UHPC1 since the particular cementitious matrix of
UHPC limits the slag pozzolanic reaction to a great extent, with the result that beyond 90 days only a small amount of slag is avail-able to react with portlandite. The data also show that the port-landite consumption in all UHPC mixtures increased with the progress of the hydration age. Compared to the portlandite quanti-ties at 3 days, the mass loss amounts at 90 days were reduced by about 39%, 41%, 21% and 37% for UHPC1, UHPC2, UHPC3and UHPC4
respectively. The increase in slag content induces a decrease in non-evaporable water on account of the weak hydraulic activity of the slag blended matrix. FromFig. 5, it was observed that the peaks of both C-S-H and ettringite in all UHPC mixtures at 90 days were higher than that at 3 days, indicating an increase in C-S-H at the cost of portlandite because of the pozzolanic reaction
. The portlandite peaks of all the blended mixtures of UHPC are lower due to the impact of dilution and the consumption of port-landite by the pozzolanic reaction. In addition, there are different peaks of calcite, as observed inFig. 5. Some phases such MgCO3,
MnCO3and FeCO3can decompose at temperatures lower than that
of calcite. However, all the curves clearly show the decrease in cal-cite when the cement content decreases.
4.1.2. Effect of chemical activation
Fig. 6 shows the mass loss for alkali-activated and non-activated UHPC4. This figure highlights the rapid decrease in mass
for activated UHPC, at 3 and 90 days, in comparison with that of non-activated ones. The difference is clearly shown inFig. 7, where the peak corresponding to C-S-H decomposition is particularly high for activated UHPC. At 3 days, a plateau is observed for non-activated UHPC4, denoting a delay in the formation of hydrates,
for high BFS content and in the absence of any activator. Using KOH appears to promote the BFS reaction and accelerate the devel-opment of hydrates, from early age, as shown in Table 3, for UHPC4-[KOH]3. At 90 days, the measured peaks of C-S-H are
prac-tically the same for both activated and non-activated UHPCs. The activation of UHPC4increases the chemically bound water
twofold at 3 days, denoting an acceleration of the slag reaction, which consumes all the portlandite produced. Thus, the hydration reaction is rapidly stopped, which explains the low content in chemically bound water of UHPC4-[KOH]3at 90 days, in
compar-ison with the non-activated one.
The results obtained agree with those of hydration, where a second peak of heat flow appeared 16 h earlier when KOH was used, corresponding to the reaction of slag.
4.1.3. Effect of thermal activation
In order to obtain the same performances of UHPC1at 90 days,
concretes with high slag content were thermally activated. As expected, a great mass loss was observed, at early age, for -0.35 -0.25 -0.15 -0.05 0.05 0 300 600 900 1200 UHPC1 UHPC2 UHPC3 UHPC4 Temperature (°C) DTG (%/min) C-S-H & Eringite Portlandite Calcite
Fig. 5. DTG for UHPC mixtures at 90 days.
Mass loss percentages (%) for reaction products from TGA analysis of UHPC mixtures.
Mixture designation Chemically bound water Portlandite Calcite
3 days 90 days 3 days 90 days 3 days 90 days
UHPC1 3.30 4.80 1.42 0.86 3.90 5.30 UHPC2 3.10 4.90 1.35 0.80 3.00 3.30 UHPC3 2.60 4.80 0.93 0.73 2.90 3.00 UHPC4 2.10 4.10 0.35 0.22 2.80 2.50 UHPC4-[KOH]3 4.40 3.80 0.00 0.00 4.20 1.80 UHPC3-T 4.80 0.00 1.20 UHPC4-T 3.70 0.00 0.20
thermally-activated UHPCs, in comparison with non-activated UHPC1 (seeFig. 8). Later, the curves have a similar trend.Fig. 9
shows that this increase corresponds particularly to the dehydra-tion of C-S-H, as thermal activadehydra-tion promotes cement hydradehydra-tion and the pozzolanic reaction. This results in increasing the C-S-H content of UHPC3and UHPC4, by circa 6 and 4 times,
respec-tively. UHPC3-T and UHPC4-T contain respectively 4 and 4.6 times
more C-S-H than UHPC1. FromTable 3, it can be seen that even if
the chemically bound water measured is the same for UHPC3-T
and UHPC1(4.8%), that of UHPC4is lower (3.7%). The high content
of slag in the latter affects the hydration progress, despite the application of thermal activation, which could result in a decrease in compressive strength.
As for chemical activation, thermal activation promotes cement and mineral additions reactions, which increase portlandite con-sumption.Table 3shows the total consumption of portlandite in UHPC3-T and UHPC4-T and the presence of a small quantity of
cal-cite, proportional to their cement contents.
The total porosity of each UHPC specimen was measured at 3 and 90 days and analyzed regardless of the slag content and the chemical and thermal activations applied. Results are summarized inTable 4.
4.2.1. Effect of slag content
Table 4shows that the porosity of UHPC1is very low (5.45%)
even at 3 days. As mentioned earlier, the essential cementitious compound in UHPC1 is silica fume. At larger amounts of silica
fume, e.g. 25%, the capillary porosity is low. As a rule, silica fume improves the packing density of UHPC in two ways: i) its filler impact through its finer particles that fill the voids between cement particles and the spaces between cement particles and aggregate, and ii) the pozzolanic impact due to the fact that the sil-ica fume reacts with portlandite to form further C–S–H gel result-ing in an additional decrease in both pore diameter and capillary porosity through hydration . For UHPC2, the total porosity
dropped by 18% compared to that of UHPC1at 3 days. The
hetero-geneous nucleation caused by the fineness of slag particles prevails over the latent reaction of slag, which results in the acceleration of hydrationand decreases UHPC porosity. In contrast, when the slag content was high, the total porosity also increased. For UHPC3
and UHPC4, the porosity was enhanced by 1.9 and 2.3 times
respec-tively, in comparison with UHPC1. This increase in the porosity of
UHPC specimens cured at 3 days is due to the latent reactivity of slag. The higher slag inclusion increases the porosity of UHPC spec-imens cured at 3 days on account of the latent reactivity of slag. This decelerates the hydration reaction of blended slag mixtures and postpones the formation of hydrates, which induces an increase in the number of coarse pores and hence in the total porosity[20,45].
At advanced ages the porosity of the blended slag mixture tends to be lower than that of the Portland cement mixture. The reaction -7 -5 -3 -1 1 0 300 600 900 1200 UHPC4-3 days UHPC4-90 days UHPC4-[KOH]3-3 days UHPC4-[KOH]3-90 days Temperature (°C) Mass Loss (%)
Fig. 6. TGA for UHPC4mixtures with and without chemical activation.
-0.3 -0.1 0.1
0 300 600 900 1200
UHPC4-3 days UHPC4-90 days UHPC4-[KOH]3-3 days UHPC4-[KOH]3-90 days
Temperature (°C) DTG ( %/m in) Portlandite Calcite C-S-H & Eringite
Fig. 7. DTG for UHPC4mixtures with and without chemical activation.
-10 -8 -6 -4 -2 0 0 300 600 900 1200 UHPC3-T UHPC4-T UHPC1-90 days Temperature (°C) Mass Loss (%)
Fig. 8. Comparison of TGA curves for thermally-activated UHPC3 and UHPC4
mixtures with the reference one at 90 days.
-1.2 -1 -0.8 -0.6 -0.4 -0.2 0 0.2 0 300 600 900 1200 UHPC3-T UHPC4-T UHPC1-90 days DTG (%/min) Temperature (°C) C-S-H & Eringite Calcite Portlandite
Fig. 9. Comparison of DTG curves for thermally-activated UHPC3 and UHPC4
mixtures with the reference one at 90 days.
Total porosity of UHPC specimens.
Mixture designation Total porosity (%)
3 days 90 days UHPC1 5.45 4.81 UHPC2 4.47 3.85 UHPC3 10.51 2.51 UHPC4 12.57 4.04 UHPC4-[KOH]3 7.72 4.14 UHPC3-T 2.64 UHPC4-T 4.09
of slag and C-S-H fills capillary pores and refines the structure, which increases the fine pores of blended mixtures[46,47].
At 90 days, the total porosity of UHPC1and UHPC2decreased by
circa 12% and 14%, respectively, in comparison with that at 3 days. For slag contents of 50% and 80%, the porosity decreased by 4 and 3 times, respectively. This result highlights the latent reaction of slag, which has a beneficial effect in the long term. Thus, the slag reaction generates hydration products that fill the large pores con-tinuously at a prolonged hydration age and significantly decreases the concrete porosity[45,48].
4.2.2. Effect of chemical activation
As observed, adding KOH decreases the total porosity of UHPC4
by 39% at 3 days. The porosity measured at 90 days changed slightly. As is well-known, AAS paste has a finer matrix system than cement paste because for the same water-to-binder ratio, the hydration products have more gel pores and the pastes have fewer capillary pores. Several studies have established that when a suitable chemical activator is used, the porosity of alkali-activated slag paste is lower, with smaller pores and a higher pro-portion of micro pores, while the propro-portion of capillary pores is less than in Portland cement paste[49–51]. The microstructure evolution of hydrating AAS paste is governed by rapid alterations at early ages, and latent evolution later. This correlates well with the quick setting of the AAS mixture, and its slow strength devel-opment at later ages[31,36].
4.2.3. Effect of thermal activation
Table 4shows that the effect of thermal activation was more pronounced than that of chemical activation on the porosity of the thermally-activated UHPC3 and UHPC4 mixtures at 3 days
whereas at 90 days there is no clear impact on the porosity apart from a slight decrease when compared to UHPC1. This was linked
with the slag content; the higher the slag content of thermally-activated UHPC, the more porosity decreases. The high tempera-ture accelerates the hydration of cement and significantly pro-motes the slag reaction during early ages, making the composite binder highly compact. These results agree with the TGA observa-tions, that demonstrate the increase in C-S-H content when UHPCs are thermally activated. These hydrates fill voids, improve the packing density of concrete and greatly decrease its porosity. 4.3. Mechanical properties
In this section, the flexure, compressive and splitting tensile strengths are explored for the different UHPCs studied. The cited parameters were analyzed regardless of BFS content and activation methods, as the mechanical properties of UHPC depend on the cur-ing regime.
4.3.1. Effect of slag content
The incorporation of different amounts of slag in blended mix-tures of UHPC results in different flexure and compressive strengths, as illustrated byFigs. 10and11, respectively.
Figs. 10 and 11show that the strength gains of UHPC2in flexion
are 6%, 4%, 13% and 4% whereas the gains in compression ratios are 2.8%, 6%, 1.4% and 1.2% for 3, 7, 28 and 90 days respectively. If we focus on compressive strength, we note that the substitution of 30% of cement with BFS induces a pronounced increase at early age (3 and 7 days) in comparison with 28 and 90 days. There are two possible reasons for this result: i) the high superplasticizer dosage of UHPC1, compared to UHPC2, which restricts the
hydra-tion reachydra-tion of cement particles and delays the formahydra-tion of hydrates. This results in decreasing compressive strength, particu-larly at early age (3 days); ii) the beneficial effect of BFS particles on concrete hydration and hardening. This effect, due to the high
specific area of BFS, is twofold: a physical effect, by improving the packing density of UHPC, and a chemical effect by activating the cement hydration. Thanks to their fineness, BFS particles fill voids between cement grains and those between quartz sand ones, which enhances the bond strength between the components of the matrix skeleton [21,52] and intensifies the interfacial transition zone of the aggregate-cement paste. In addition, BFS particles, like SF ones, act as heterogeneous nucleation sites, thereby accelerating the hydration of cementand the formation of hydrates, neces-sary for strength development. The results are in accordance with those of thermogravimetric analysis. The low density C-S-H gel that is formed fills the capillary pores, thus decreasing the total porosity of UHPC2by 18% at 3 days, as shown inTable 4.
At later ages (28 and 90 days) the difference between UHPC1
and UHPC2is reduced, and the compressive strength of the latter
slightly exceeds that of the former. This trend can be explained by the low water content of UHPC, which restricts the long-term SF and BFS reactions since, unlike ordinary and high performance concretes, the portlandite formed in UHPC is reduced. As port-landite is necessary for the pozzolanic reaction of SF and BFS, its scarcity decreases their reactivity.
In order to show the filler effect of slag in improving packing density and hence the compressive strength of concrete, limestone filler was incorporated as a partial substitution of cement (30%) and the concrete was compared to that with slag.Figs. 12 and 13
show respectively the flexure and compressive strength of UHPC2
based on slag and limestone filler.
Despite its lower specific area, in comparison with limestone fil-ler, slag confers more compressive strength at all curing ages. This
Fig. 10. Flexure strength of studied UHPCs.
0 20 40 60 80 100 120 140 160 180 0 20 40 60 80 100 UHPC1 UHPC2 UHPC3 UHPC4 Compressive strength (MPa) Time (Days)
result highlights the slight reactivity of slag at early age, which compensates for the loss of strength that should occur because of decreasing specific area. Limestone filler, despite its high specific area, is considered as an inert mineral material. Its effect consists in increasing the compressive strength at early age by heteroge-neous nucleation, while slag could play a complex role consisting in filling voids between cement particles, improving compressive strength by heterogeneous nucleation in addition to its chemical effect through its latent reactivity at early age.
With high BFS content, the decrease in compressive and flexure strengths is significant, particularly at early age. As shown in
Fig. 10, the drop in compressive strength of UHPC3is 26%, 12%,
11% and 7% whereas for UHPC4 it is 66%, 37%, 22% and 27% at
3,7, 28 and 90 days, respectively. As explained in our recent study
, at early age, the dilution effect of BFS particles prevails over the effect of heterogeneous nucleation. This results in a high liq-uid–solid ratio, delaying the hardening of UHPC and its strength development. According to thermogravimetric analysis, at 3 days, the rates of hydrates and portlandite formed are very low, denoting the delay of cement hydration and the latent reaction of slag, mak-ing the UHPC microstructure more porous and reducmak-ing the com-pressive strength. At later ages (28 and 90 days), the difference between UHPC1 and UHPC3 decreases, denoting the progress of
the pozzolonic reaction of SF and BFS. For UHPC4, the compressive
strength, despite its rapid increase between 3 and 7 days, is the same at 28 and 90 days. This trend shows that the hydration reac-tion of solid components is postponed after 28 days and the rate of hydrates formed is low. Indeed, with a high BFS and a low water content, the amount of portlandite produced is limited and is not enough for the pozzolanic reaction of SF and BFS. This reduces the C-S-H content and decreases the compressive strength, despite the refinement of the microstructure.
Fig. 14shows the splitting tensile strength of different UHPCs at 3 and 28 days. All the manufactured UHPCs have a splitting tensile strength at 28 days exceeding 8 MPa, despite the absence of fibers. This result is very interesting, as the tensile strength is a key parameter in UHPC mixture design.
Even if a low BFS content does not greatly affect the concrete tensile strength, for 50% of cement substitution a decrease in strength of 10% and 13% was measured at 3 and 28 days, respec-tively. The drop in tensile strength is particularly pronounced for concrete with 80% of BFS at 3 days, reaching 68%. This result agrees with that of compressive strength.
The same factors influencing the compressive strength of the tested UHPCs are presented below to explain the effect of BFS con-tent on the splitting tensile strength, even if the latter seems less sensitive than the former.
4.3.2. Effect of chemical activation
As mentioned earlier, the original concentration of the alkaline activator used here, [KOH]1, was calculated to compensate for the
lack of alkalis caused by the substitution of cement. The concentra-tion of KOH needs to be high to improve the early age properties of blended UHPCs. Therefore, we will focus on UHPC4, where the
rate of cement substitution is high. Thus, a large quantity of KOH (proportional to the BFS content) can be added. To ensure the required compressive strength of UHPC4, the concentration of
[KOH]1was increased up three times ([KOH]3). This is considered
as the optimal concentration, even if more hydroxide potassium is necessary to improve the early compressive strength of UHPC4,
in order to reach that of reference UHPC, since more KOH strongly affects the workabilityof concrete and has a negative effect on its implementation and then on its compressive strength.
Figs. 15 and 16depict the variation of both flexure and com-pressive strengths of KOH-activated UHPCs with 80% slag (UHPC4).
As shown inFig. 15, the flexure strength increases proportion-ally to the activator concentration, denoting the regularity and the high density of the interfacial transition zone between the bin-der and the aggregate in alkali-activated slag mixtures. This was helpful for increasing the bond strength of alkali-activated concretes as in presence of alkalis, BFS particles react rapidly, pro-moting the formation of hydrates, which explains the high con-sumption of portlandite for UHPC4-[KOH]3 (Section 4.1.2). The
hydrates formed fill the porosity and improve the properties of the transition zone in [KOH]-activated UHPCs. This results in an increase in flexure strength.
Like flexure strength, compressive strength is improved by chemical activation, particularly at early age and with a high con-centration of alkaline activator. For [KOH]3, the measured growth
of compressive strength was nearly 42% at 3 days whereas at 7, 0 5 10 15 20 25 UHPC2 UHPC-Filler
3 Days 7 Days 28 Days 90 Days
F le x u re st re n g th ( M P a )
Fig. 12. Flexure strength of UHPC2with slag and limestone filler.
0 25 50 75 100 125 150 175 UHPC2 UHPC-Filler
3 Days 7 Days 28 Days 90 Days
Fig. 13. Compressive strength of UHPC2with slag and limestone filler.
0 2 4 6 8 10 12 3 Days 28 Days UHPC3
UHPC1 UHPC2 UHPC4
28 and 90 days, the strength gain reached about 14%, 3% and 14%, as shown onFig. 16. This trend is in accordance with that of previ-ous studies, emphasizing the dosage of activating agent as a para-mount factor in improving the early age performance of blended mixtures[54–57].
The presence of a high concentration of KOH increases the solu-tion’s pH (i.e. higher alkalinity and correspondingly higher concen-tration of OH–ions), which increases the dissolution ability of both Si and Al ions by destroying the SiAO and AlAO bonds in the slag glass matrix. This is followed by the precipitation of hydrated products with low solubility, such as calcium silicates, calcium alu-minates, and magnesium aluminate. Then, steady ettringite is formed as a result of the interaction between Ca and Al. As a com-bined result of rising pH and ettringite formation, hydration is accelerated, increasing hydrate formation and improving the compressive strength of concrete at early age . The result obtained agrees with those of thermogravimetric analysis and porosity: the DTG curves clearly show the great increase in C-S-H at 3 days when KOH is added, decreasing the total porosity of UHPC4by 39%.
4.3.3. Effect of thermal activation
In order to reach the required compressive strength of reference concrete at 90 days, UHPC3and UHPC4were thermally-activated.
The results of flexure and compressive strengths in comparison with UHPC1at 90 days are shown inFigs. 17 and 18, respectively.
In comparison with non-activated blended UHPCs, the flexure and compressive strength of both UHPC3-T and UHPC4-T increased
substantially. This result shows the important role of thermal acti-vation in accelerating the hydration process and producing hydrates, particularly in presence of BFS and SF, which improves the packing density and decreases the concrete’s porosity. This results in increasing the mechanical properties of UHPC.
As observed inFig. 18, thermal activation increases the com-pressive strength at 3 days of UHPC3and UHPC4by 1.7 and 3 times,
respectively. The temperature accelerates the reaction of the solid components of concrete, particularly BFS. Thus, the higher the amount of slag, the higher the apparent hydration activation energy[31,32]. At 90 days, the compressive strength increase is circa 16% and 20% respectively for UHPC3and UHPC4. This result
shows that contrary to ordinary and high performance concretes, thermal activation improves the mechanical properties of UHPC at later age. For the former with thermal activation, there is not enough time for hydrated products to be regularly arranged inside the pores of the hardened paste, which enlarges the capillary pores and then decreases the later strength. This phenomenon is known as crossover impact[33,35]. For UHPC, there is not enough water for complete concrete hydration, which enables the development of compressive strength at later age. Therefore, the high tempera-ture compensates for the lack of water, by activating the solid com-ponents, particularly the more sensitive ones (BFS). This results in a high consumption of portlandite (0% for thermally-activated UHPC) by mineral admixtures, inducing a high production of hydrates which fill the pores and improve the packing density of UHPC. The porosity drops and the compressive strength increases. As already mentioned, the objective of thermal activation is to reach the compressive strength of UHPC1at 90 days. This objective
was reached for UHPC3and its compressive strength exceeded that
of reference concrete by 7%, denoting the effectiveness of the acti-vation mode applied (temperature and duration). For UHPC4,
ther-mal activation improved the compressive strength but without reaching that of reference concrete (-12.5%) as the low cement con-tent combined with the high water absorption of SF and BFS strongly affect the compressive strength, and thermal activation at 90°C for 48 h did not counterbalance this drop. Therefore, the temperature should be increased or the duration should be extended to compensate for the decrease in compressive strength in presence of a high BFS content. However, the environmental footprint of this activated UHPC has to be assessed, despite its low cement content. Another activation mode, without increasing temperature or duration, could be investigated, combining chemi-cal and thermal activation.
0 5 10 15 20 25 UHPC4 UHPC4-[KOH]1 UHPC4-[KOH]2 UHPC4-[KOH]3
3 Days 7 Days 28 Days 90 Days
Fig. 15. Flexure strength of KOH-activated UHPC4.
0 20 40 60 80 100 120 140 UHPC4 UHPC4-[KOH]1 UHPC4-[KOH]2 UHPC4-[KOH]3
3 Days 7 Days 28 Days 90 Days
Fig. 16. Compressive strength of KOH-activated UHPC4.
0 5 10 15 20 25 Flexure strength (MPa)
UHPC1-90 days UHPC3-T UHPC4-T
Fig. 17. Comparison of flexure strengths of thermally-activated UHPC3and UHPC4
4.3.4. Effect of combined chemical and thermal activation
The combined activation mode consists in using chemical and thermal activation sequentially. In our case, UHPC4-[KOH]3 was
demolded after 24 h and thermally-activated for 48 h, as detailed previously. The results of flexure and compressive strengths at 3, 28 and 90 days are shown inFigs. 19 and 20, respectively.
Figs. 19 and 20show clearly that the effect of chemical activa-tion with [KOH]3 is negligible, as the measured compressive
strength does not exceed that of UHPC4-T. This result highlights
two interesting points: i) even if [KOH]3improves the compressive
strength of UHPC4at 3 days, this improvement is negligible at 1
day, as the concrete has a high superplasticizer content, which decelerates the hydration reaction of cement and hence that of activated slag; ii) thermal activation, applied at 1 day, ensures an activation of all silicon solid components, which accelerates their hydration reaction and induces a pronounced increase in strength. In addition, the hydrates formed in thermally-activated UHPC are denser than those formed with chemical activation. Therefore, in our case study, it is not interesting to combine chemical and ther-mal activation.
The work carried out allows us to draw the following conclusions:
– With 30% of slag, the heterogeneous nucleation effect of BFS particles prevails over the effect of dilution. This results in an acceleration of the cement hydration reaction and consequently that of mineral admixtures (SF and BFS), which increases the amount of hydrates produced. The latter improve the packing density of concrete and decrease its porosity. Therefore, the compressive strength increases.
In addition to the compressive strength enhancement, BFS par-ticles improve the UHPC workability by their filling and lubrica-tion roles, which decreases the superplasticizer content. This reduces the environmental impact and the cost of UHPC2 in
comparison with UHPC1.
– For high BFS content (50% and 80%), the dilution effect prevails over the heterogeneous nucleation effect. The compressive strength of UHPC3and UHPC4increased slightly, denoting the
low portlandite content, which results in fewer hydrates. Despite the physical effect (filling pores and improving the packing density) of BFS, the lack of water and portlandite restrict the pozzolanic reaction of SF and BFS, which decreases the mechanical performance of blended UHPC in comparison with the reference one.
– Alkaline activation with [KOH]3increases the dissolution of Si
and Al ions by breaking the SiAO and AlAO bonds in the slag glass, which promotes the BFS reaction. This increases the amount of C-S-H, decreasing porosity and improving the com-pressive strength of UHPC4at early age.
– Thermal activation increases the reaction of solid components and accelerates their hydration, which increases the consump-tion of portlandite. Therefore, more hydrates are formed, filling the porosity, improving the packing density of UHPC and enhancing its mechanical performance. For UHPC3-T, the
ther-mal activation parameters chosen ensured the required com-pressive strength. However, with 90°C and 48 h of activation, the compressive strength of UHPC4-T was 12.5% less than that
of UHPC1at 90 days, due to the lack of water and the high BFS
content. In order to improve the compressive strength of UHPC4,
higher temperatures or longer durations have to be explored, as the combined chemical and thermal activation was not enough to compensate for the drop in strength.
The authors would like to address their thanks to Jérôme Carriat for his technical help in manufacturing and characterizing the concretes. 0 25 50 75 100 125 150 175 Compr e ssi ve str e ngth (MPa)
UHPC1-90 days UHPC3-T UHPC4-T
Fig. 18. Comparison of compressive strengths of thermally-activated UHPC3and
0 5 10 15 20 25 30 UHPC4 UHPC4-[KOH]3T
3 Days 28 Days 90 Days
Flexure strength (MPa)
Fig. 19. Flexure strength of chemically and thermally-activated UHPC4mixtures.
0 25 50 75 100 125 150 175 UHPC4 UHPC4-[KOH]3T
3 Days 28 Days 90 Days
Fig. 20. Compressive strength of chemically and thermally-activated UHPC4
 E. Fehling, M. Schmidt, J. Walraven, T. Leutbecher, S. Frӧhlich, Ultra-high performance concrete UHPC: Fundamentals-Design-Examples, Wilhelm Ernst & Sohn, 10245 Berlin, Germany, 2014.
V. Corinaldesi, G. Moriconi, Mechanical and thermal evaluation of ultra high performance fiber reinforced concretes for engineering applications, Constr. Build. Mater. 26 (2012) 289–294.
M. Laneza, M.N. Oudjita, A. Zenatia, K. Arroudj, A. Bali, Micro Environ. Concr. Phys. Proced. 21 (2011) 159–165.
M.A.A. Aldahdooh, N.M. Bunnori, M.A.M. Johari, Influence of palm oil fuel ash on ultimate flexural and uniaxial tensile strength of green ultra-high performance fiber reinforced cementitious composites, Mater. Des. 54 (2014) 694–701.
D. Mostofinejad, M.R. Nikoo, S.A. Hosseini, Determination of optimized mix design and curing conditions of reactive powder concrete (RPC), Constr. Build. Mater. 123 (2016) 754–767.
A. Beglarigale, H. Yazıcı, Pull-out behavior of steel fiber embedded in flowable RPC and ordinary mortar, Constr. Build. Mater. 75 (2015) 255–265. P. Richard, M. Cheyrezy, Composition of reactive powder concretes, Cem.
Concr. Res. 25 (1995) 1501–1511.
D.-Y. Yoo, N. Banthia, Mechanical properties of ultra-high-performance fiber-reinforced concrete: a review, Cem. Concr. Compos. 73 (2016) 267–280.  P. Mounanga, K. Cherkaoui, A. Khelidj, M. Courtial, M.-N. de Noirfontaine, F.
Dunstetter, Extrudable Reactive Powder Concretes: Hydration, shrinkage and transfer properties. Europ. J. Environ. Civ. Eng. 16 (1) (2012) 1–20. M. Courtial, M.-N. de Noirfontaine, F. Dunstetter, M. Signes-Frehel, P.
Mounanga, K. Cherkaoui, A. Khelidj, Effect of polycarboxylate and crushed quartz in UHPC: microstructural investigation, Constr. Build. Mater. 44 (2013) 699–705.
D. Wang, C. Shi, Z. Wu, J. Xiao, Z. Huang, Z. Fang, A review on ultra high performance concrete: Part II. Hydration, microstructure and properties, Constr. Build. Mater. 96 (2015) 368–377.
A.M. Rashad, D.M. Sadek, H.A. Hassan, An investigation on blast-furnace slag as fine aggregate in alkali-activated slag mortars subjected to elevated temperatures, J. Clean. Prod. 112 (2016) 1086–1096.
H. Yazıcı, H. Yig˘iter, A.Sß. Karabulut, B. Baradan, Utilization of fly ash and ground granulated blast furnace slag as an alternative silica source in reactive powder concrete, Fuel 87 (2008) 2401–2407.
E. Aprianti, P. Shafigh, R. Zawawi, Z.F. Abu, Hassan, introducing an effective curing method for mortar containing high volume cementitious materials, Constr. Build. Mater. 107 (2016) 365–377.
F. Sajedi, Effect of curing regime and temperature on the compressive strength of cement-slag mortars, Constr. Build. Mater. 36 (2012) 549–556.
C. Li, H. Sun, L. Li, A review: The comparison between alkali-activated slag (Si +Ca) and metakaolin (Si+Al) cements, Cem. Concr. Res. 40 (2010) 1341–1349. P. Lawrence, M. Cyr, E. Ringot, Mineral admixtures in mortars. Effect of inert materials on short-term hydration, Cem. Concr. Res. 33 (2003) 1939–1947. R. Yu, P. Spiesz, H.J.H. Brouwers, Development of an eco-friendly Ultra-High
Performance Concrete (UHPC) with efficient cement and mineral admixtures uses, Cem. Concr. Compos. 55 (2015) 383–394.
 P.E. Holthuizen, Chloride ingress of carbonated blast furnace slag cement mortars, Section of Materials and Environment (Master Thesis), Delft University of Technology, Netherlands, 2016.
 J. Zhou, G. Ye, K. van Breugel, Hydration process and pore structure of portland cement paste blended with blast furnace slag, in: Proceedings of the 6th International Symposium on Cement & Concrete, Canmet, 2006, pp. 1–7. H. Yazıcı, M.Y. Yardımcı, S. Aydın, A.S. Karabulut, Mechanical properties of
reactive powder concrete containing mineral admixtures under different curing regimes, Constr. Build. Mater. 23 (2009) 1223–1231.
 S. Gupta, Development of ultra-high performance concrete incorporating blend of slag and silica fume as cement replacement, Int. J. Civ. Struct. Eng. Res. 2 (1) (2014) 35–51.
C. Shi, D. Wang, L. Wu, Z. Wu, The hydration and microstructure of ultra-high-strength concrete with cement–silica fume–slag binder, Cem. Concr. Compos. 61 (2015) 44–52.
S.A. Bernal, R. Mejía de Gutiérrez, A.L. Pedraza, J.L. Provis, E.D. Rodriguez, S. Delvasto, Effect of binder content on the performance of alkali-activated slag concretes, Cem. Concr. Res. 41 (2011) 1–8.
F. Sajedi, H. Abdul Razak, The effect of chemical activators on early strength of ordinary Portland cement-slag mortars, Constr. Build. Mater. 24 (2010) 1944– 1951.
X. Wu, W. Jiang, D.M. Roy, Early activation and properties of slag cement, Cem. Concr. Res. 20 (1990) 961–974.
M. Kovtun, E.P. Kearsley, J. Shekhovtsova, Chemical acceleration of a neutral granulated blast-furnace slag activated by sodium carbonate, Cem. Concr. Res. 72 (2015) 1–9.
B.S. Gebregziabiher, R. Thomas, S. Peethamparan, Very early-age reaction kinetics and microstructural development in alkali-activated slag, Cem. Concr. Compos. 55 (2015) 91–102.
E. Altan, S.T. Erdog˘an, Alkali activation of a slag at ambient and elevated temperatures, Cem. Concr. Compos. 34 (2012) 131–139.
 W. Chen, Hydration of slag cement: Theory, modeling, and application, University of Twente (Doctoral Thesis), The Netherlands, 2007.
 F. Sajedi, H. Abdul Razak, Effects of thermal and mechanical activation methods on compressive strength of ordinary Portland cement–slag mortar. Mater. & Des. 32 (2011) 984-995.
 F. Sajedi, H. Abdul Razak, Thermal activation of ordinary Portland cement–slag mortars. Mater. Des. 31 (2010) 4522–4527.
A. Sadrekarimi, Development of a light weight reactive powder concrete, J. Adv. Concr. Technol. 2 (3) (2004) 409–417.
A. Bougara, C. Lynsdale, K. Ezziane, Activation of Algerian slag in mortars, Constr. Build. Mater. 23 (2009) 542–547.
C.C. Castellano, V.L. Bonavetti, H.A. Donza, E.F. Irassar, The effect of w/b and temperature on the hydration and strength of blast furnace slag cements, Constr. Build. Mater. 111 (2016) 679–688.
O.M. Abdulkareem, A. Ben, Fraj, M. Bouasker, A. Khelidj, Mixture design and early age investigations of an environmentally friendly UHPC, Constr. Build. Mater. 163 (2018) 235–246.
M. Regourd, F. Gautier, Behaviour of concretes subjected to accelerated hardening (in French), J. Constr. Mater. 725 (1980) 240–248.
 M.H. Kazemi-Kamyab, Autogenous shrinkage and hydration kinetics of Sh-UHPFRC under moderate to low temperature curing conditions (Thesis), EPFL, 2013.
 P. Francisco, Déformations différées des bétons fibrés à ultra hautes performances soumis à un traitement thermique (Thesis), ENS Cachan, 2014 (in French).
 M. Ashraf, A.N. Khan, Q. Ali, J. Mirza, A. Goyal, A.M. Anwar, Physico-chemical, morphological and thermal analysis for the combined pozzolanic activities of minerals additives, Const. Build. Mater. 23 (2009) 2207–2213.
N.E. Khalifa, M. Bouasker, P. Mounanga, N. Benkahla, Physico-chemical study of cementitious materials based on binary and ternary binders, Chem. Mater. Res. 4 (2013) 19–24.
S. Kourounis, S. Tsivilis, P.E. Tsakiridis, G.D. Papadimitriou, Z. Tsibouki, Properties and hydration of blended cements with steelmaking slag, Cem. Concr. Res. 37 (2007) 815–822.
M. Heikal, O.K. Al-Duaij, N.S. Ibrahim, Microstructure of composite cements containing blast-furnace slag and silica nano-particles subjected to elevated thermally treatment temperature, Constr. Build. Mater. 93 (2015) 1067–1077. C. Shi, D. Wang, L. Wu, Z. Wu, The hydration and microstructure of ultra high-strength concrete with cement-silica fume-slag binder, Cem. Concr. Compos. 61 (2015) 44–52.
L. Rengguang, D. Shidong, Y. Peiyu, Microstructure of hardened complex binder pastes blended with slag, J. Chin. Ceram. Soc. 43 (5) (2015) 610–618. O.R. Ogirigbo, L. Black, Influence of slag composition and temperature on the
hydration and microstructure of slag blended cements, Cem. Concr. Compos. 126 (2016) 496–507.
S.N. Ghosh, Advanced in Cement Technology: Chemistry, Manufacture, and Testing, Tech Books International, New Delhi, India, 2002.
 A.A. Ramezannianpour, Cement Replacement Materials: Properties, Durability, Sustainability, Springer-Verlag, Berlin Heidelberg, Germany, 2014.
C. Shi, D. Roy, P. Krivenko, Alkali-Activated Cements and Concretes, Taylor and Francis Group, USA, 2006.
 F. Collinsa, J.G. Sanjayan, Effect of pore size distribution on drying shrinkage of alkali-activated slag concrete, Cem. Concr. Res. 30 (2000) 1401–1406. S.L. Yang, S.G. Millard, M.N. Soutsos, S.J. Barnett, T.T. Le, Influence of aggregate
and curing regime on the mechanical properties of ultra-high performance fibre reinforced concrete (UHPFRC), Constr. Build. Mater. 23 (2009) 2291– 2298.
R. Siddique, Waste Materials and By-Products in Concrete, Springer-Verlag, Berlin Heidelberg, 2008.
K.V. Schuldyakov, L.Ya. Kramar, B.Ya. Trofimov, The properties of slag cement and its influence on the structure of the hardened cement paste, Proc. Eng. 150 (2016) 1433–1439.
A. Gruskovnjak, B. Lothenbach, L. Holzer, R. Figi, F. Winnefeld, Hydration of alkali-activated slag: comparison with ordinary Portland cement, Adv. Cem. Res. 18 (3) (2006) 119–128.
M. Heikal, M.Y. Nassar, G. El-Sayed, S.M. Ibrahim, Physico-chemical, mechanical, microstructure and durability characteristics of alkali activated Egyptian slag, Constr. Build. Mater. 69 (2014) 60–72.
B.S. Gebregziabiher, R. Thomas, S. Peethamparan, Temperature and activator effect on early-age reaction kinetics of alkali-activated slag binders, Constr. Build. Mater. 113 (2016) 783–793.
C. Bilim, C.D. Atisß, Alkali activation of mortars containing different replacement levels of ground granulated blast furnace slag, Constr. Build. Mater. 28 (2012) 708–712.
D. Ravikumar, N. Neithalath, Effects of activator characteristics on the reaction product formation in slag binders activated using alkali silicate powder and NaOH, Cem. Concr. Compos. 34 (2012) 809–818.
H. Yazıcı, M.Y. Yardımcı, H. Yig˘iter, S. Aydın, S. Türkel, Mechanical properties of reactive powder concrete containing high volumes of ground granulated blast furnace slag, Cem. Concr. Compos. 32 (2010) 639–648.